Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses


 Emmeline Baldwin
 1 years ago
 Views:
Transcription
1 International Journal of Adhesion & Adhesives 20 (1999) International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses John A. Nairn Department of Material Science and Engineering, University of Utah, 122 S. Central Campus Drive, Room 304 Salt Lake City, UT , USA Received 6 November 1996 Abstract The mode I energy release rate, including the effect of residual stresses, was evaluated for both adhesive and laminate double cantilever beam specimens. The energy release rate can be partitioned into a mechanical term and a residual stress term in beam theory. The beamtheory mechanical term is not very accurate, but can be corrected by a slight modification to a previous correction factor. This correction factor accounts for crack tip rotation of the specimen arms. The beamtheory residual stress term is very accurate for a wide range of specimen geometries; it can be used without correction. The consequence of ignoring residual stresses is that one measures an apparent toughness instead of a true toughness. The error between the apparent toughness and true toughness can be calculated for a given specimen geometry and amount of residual stresses. Such errors can be large and are often larger than the correction required for cracktip rotation effects. In double cantilever beam specimens used to study laminate delamination, the errors are large when the delaminating arms, considered by themselves, are unsymmetric laminates. Some experimental methods are suggested which can used to correct for residual stress effects. Keywords: Adhesive Toughness, Fracture Mechanics, Residual Stresses, Delamination 1. Introduction Since the work of Mostovoy, Ripling, et al. [1 3], the double cantilever beam (DCB) specimen geometry has been a popular method for measuring the fracture toughness of adhesive bonds and delamination fracture toughness of composite laminates. There are existing standard protocols for mode I testing of both adhesive bonds [4] and laminate delamination [5]. The same specimen geometry with modified loading methods can be used for the study of mode II and mixed mode fracture as well [6, 7]. There are ongoing efforts to refine adhesive fracture and delamination methods to give the best possible results [8]. These standards, however, do not address methods for dealing with residual stresses. When adhesive joints are cured, or laminates are processed, at high temperature and then cooled to room temperature, residual stresses will inevitably be present. These stresses can arise either from differential thermal shrinkage between the components of the specimen or from chemical shrinkage of the adhesive or composite matrix resins. When a crack grows in a specimen with residual stresses, the residual stresses can contribute to the total amount of energy released. If residual stress effects are ignored, the calculated fracture toughness will not be the true fracture toughness. Instead, it will be an apparent toughness that includes a specimen property (the amount of residual stresses) within the desired material property (the toughness). When such an apparent toughness is used for prediction of failure in adhesive joints that have different levels of residual stresses, those predictions will not be correct. Furthermore, the most common residual stress effect in adhesive DCB specimens is for Tel: ; fax: address: (J.A. Nairn) /00/$see front matter c 2000 Elsevier Science Ltd. All rights reserved.
2 60 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) the apparent toughness to be larger than the true toughness. Thus, adhesive designs based on such nonconservative apparent toughnesses could lead to premature failure. This paper describes a mode I energy release rate analysis for crack growth in adhesive DCB specimens and laminate delamination specimens. The thermoelastic energy release rate analysis uses linearelastic beam theory. Largedisplacement, endblock loading, and plasticity effects were ignored, but these effects could be included by methods developed previously for delamination [7, 9] and adhesive fracture [10] analysis. The crack is assumed to propagate straight; for adhesives, it is therefore assumed to remain in the middle of the adhesive as a cohesive mode I fracture. The energy release rate can be partitioned into two terms a term involving mechanical loads and a term involving residual stresses. The accuracy of each term was studied by extensive finite element calculations. As observed in previous work, the beamtheory mechanical term is inaccurate because it ignores arm rotation at the root of the crack [7, 10, 11]. A previouslypublished correction to the mechanical term [10] is very accurate, provided it is multiplied by a numericallydetermined constant. In contrast, the beamtheory residual stress term is accurate, without correction, for a wide range of specimen geometries. From the accurate residual stress term, it is possible to calculate the error induced in the measured fracture toughness for any DCB specimen, if residual stresses are ignored. The error in adhesive DCB specimens can be significant. It gets smaller as the adhesive layer gets thinner and as the modulus ratio between the adherend and the adhesive gets larger. In laminate DCB specimens, the residual effect disappears if both arms of the DCB specimen are themselves symmetric laminates. If the arms are not symmetric laminates, the residual stress effect will generally be significant. Finally, accounting for residual stresses in analysis of DCB specimens requires knowledge of the level of residual stresses in the specimen. Some experimental methods based on calibration specimens, on observing initial beam curvatures, or on the loaddisplacement curve are discussed. The recommended method is to extrapolate the residual stress term from a properlyzeroed, loaddisplacement curve. Although the energy release rate analysis is specific for residual thermal stresses, the experimental correction method is general; it can account for any type of residual stresses. 2. General energy release rate analysis Figure 1 shows a double cantilever beam (DCB) specimen geometry used to measure the mode I toughness of adhesive bonds. In a fracture mechanics analysis of this specimen, the crack is predicted to propagate when the thermoelastic energy release rate for mode I crack growth (G I ) becomes equal to the toughness of the adhesive or the adhesive s critical energy release rate (G ). The mechanics problem is thus to find G I including the effect of residual stresses. A recent paper [12] has derived an exact result for mode I energy release rate in any composite with residual stresses: G I = d Gmech + 1 da 2 σ m α T dv V Gmech 2 (1) where G mech is the energy release rate in the absence of residual stresses, σ m is the stress tensor due to mechanical loads only, α is the positiondependent thermal expansion tensor of the composite material, and T = T s T 0 is the temperature difference between specimen test temperature (T s ) and the stressfree temperature (T 0 ). The derivative in the numerator is with respect to total crack area A. In this analysis, the adhesive DCB specimen is treated as a twophase composite with the two phases being the adhesive joint and the two adherends. Equation (1) was derived using a linear thermoelasticity analysis. It assumes residual stresses arise due to differential thermal shrinkage between the phases of the specimen under a uniform change in temperature of T [12]. Some experimental methods to correct for other types of residual stresses are discussed below. For the tractiononly loading of the adhesive DCB specimen (see Figure 1), some further results from Ref. 12 are that G mech = 1 d T 0 u m ds and σ m α T = T 0 u r ds (2) 2 da S V S
3 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) P y x v m + v r Adherend Adhesive b a La P Fig. 1. A double cantilever beam specimen used to measure the mode I toughness of adhesive bonds. The cantilever arm length is a, the total specimen length in L. Sometimes the adhesive does not extend to the end of the arms; here the adhesive stops a distance b from the ends. where T 0 is the applied surface traction, u m and u r are the displacements due to mechanical or residual stresses, respectively. For a 2D, planestress analysis (all stresses in the z direction assumed to be zero), the tractions applied to the DCB specimen are T 0 = P B δ( x x u) P B δ( x x l) (3) where P is the total applied load, B is the specimen thickness in the z direction, δ( x) is the Dirac delta function, and x u and x l are the locations of the upper and lower loading points. Substitution of this traction vector into equations (1) and (2) with da = B da, where a is the DCB specimen arm length, leads to G I = G mech + P dv 2 r da Gmech and G mech = P B where v m and v r are the load point displacements at the top loading point ( x u ) in the y direction due to mechanical or residual stresses, respectively (see Figure 1). In general, residual stresses can contribute to energy release rate either by releasing strain energy or by doing external work as the crack grows [12]. The residual stress contribution to energy release rate here is the second term in equation (4). It is immediately seen to be equal to the external work caused by changes in residual displacements (v r ) under load P at the loading points. In other words, the entire effect of residual stresses in DCB specimens is an external work effect arising from thermally induced curvature in the DCB arms. Although the full DCB specimen is a balanced structure, each DCB arm is an unbalanced, twolayer structure. As the crack grows, the unbalanced arms may curve due to residual stresses; this curvature leads to external work that causes the entire residual stress effect in G I. By equation (4), the analysis for G I is reduced to finding the loading point mechanical and residual displacements. Here one arm of the specimen will be analyzed by simple beam theory. We begin by writing the upperarm, momentcurvaturetemperature relation as dv m da κ = d2 v dx 2 = C κm + α κ T (5) where κ is beam curvature (defined as positive for curvature upwards), v is ydirection displacement, M is the applied moment, C κ is the effective beam bending compliance, and α κ is the effective beam thermalcurvature coefficient. In common adhesive specimens, the adhesive joint does not extend all the way to the loading point as shown in Figure 1 where the adhesive stops at a distance b from the end. An analysis for finding beam displacements must account for the different values of C κ and α κ in the region with adhesive and the region with no adhesive. Because b remains constant, however, as the crack propagates, the beam (4)
4 62 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) section with no adhesive makes a constant contribution to displacements that drops out when derivatives with respect to a are evaluated. In other words, G I is independent of b; for simplicity we can evaluate loadpoint displacements by setting b = 0. Integration of equation (5) for mechanical stresses only (M = P x, T = 0, and x = 0 at the loading point) or residual stresses only (M = 0, T 0) leads to where v m = 1 3 C κp a 3 and v r = 1 2 α κ T a 2 (6) Substituting loadingpoint mechanical and residual displacements into equation (4) gives C m = G I = (C m P a + C r T ) 2 (7) C κ B and C r = α κ C κ B The G I analysis has been reduced to the problem of finding the effective beam properties of the cantilever arms. Specific results for adhesive or laminate DCB specimens are given in the following two sections. In many adhesive DCB specimens, such as those with polymeric adhesives and metallic adherends, α κ T, and hence v r, will be negative. This fact seems to invalidate the residual displacement analysis because it corresponds to the upper arm displacing down and through the lower arm. The G I analysis, however, remains valid provided the total beam displacement, v = v m + v r, is positive; in other words, the analysis remains valid for any adhesive DCB test where the beam arms must be mechanically opened to induce fracture. The situation where the crack grows without v being positive corresponds to a specimen that fails due to residual stresses alone and therefore to a specimen that would not be used in a subsequent adhesive fracture test. (8) 3. Adhesive double cantilever beam specimens Analysis of adhesive DCB specimens was reduced above to finding the effective beam properties, C κ and α κ, both of which can be found by simple composite beam analyses. The preferred, but still simple, analysis is one that considers the full beam geometry or one that does not assume the adhesive is thin. The coordinates for analysis of one adhesive DCB arm are shown in Figure 2. By simple beam analysis (e.g., Ref. 13) C κ = 1 1 = (9) (EI) effective E 1 I zz,1 + E 2 I zz,2 where E i and I zz,i are the modulus and moment of inertia about the neutral axis for phase i (i = 1 for the adherend and i = 2 for the adhesive). The neutral axis is located at y N = h 1h 2 2 E 1 E 2 E 1 h 1 + E 2 h 2 (10) where h 1 and h 2 are the thicknesses of the adherend and adhesive, respectively. By the parallel axis theorem ( I zz,1 = Bh Bh 1 y N h ) 2 ( 2 and I zz,2 = Bh Bh 2 y N + h ) 2 1 (11) 2 The beam C κ can be written in a convenient form as C κ = 12 E 1 Bh 3 1 λ 2 (1 + Rλ) ( 3(1 + λ) 2 + (1 + Rλ) λ 2 + Rλ 1 ) (12) where R = E 1 E 2 and λ = h 1 h 2 (13)
5 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) h/2 B y h 1 E 1 x h/2 h 2 E 2 Fig. 2. The coordinate system used for composite beam analysis of one arm of an adhesive DCB specimen. The result for α κ is the classic Timoshenko, bimetallic strip problem [14] which can be written as ακ 6 α(1 + λ) = ( h 2 (3(1 + λ) 2 + (1 + Rλ) λ 2 + Rλ 1 )) (14) where α = α 1 α 2 is the difference in thermal expansion coefficients between the adherend and the adhesive. For typical polymeric adhesives with metallic adherends, α 1 < α 2 and T < 0 as the specimen cools from the cure temperatures to the testing temperature. For such specimens, ακ T < 0, and the residual stresses cause the beam arms to bend towards the center of the specimen. Thus, in such specimens, the residual stresses cause the beam arms to do work on the loading system. From equation (8), the mechanical and residual coefficients for determining G I are C m = 2λ 3(1 + Rλ) Bh 1 E 1 h 1 (3(1 + λ) 2 + (1 + Rλ) C r = 3E 1 h 1 α(1 + λ) ( (1 + Rλ) 3(1 + λ) 2 + (1 + Rλ) 3.1. Comparison to finite element results ( λ 2 + Rλ 1 )) (15) ( λ 2 + Rλ 1 )) (16) For judgement of the accuracy of C m and C r, a large number of finite element calculations (FEA) were done in which R was varied from 1 to 100 and λ was varied from 1 to 128. The accuracy of beam theory depends on the axial ratio of the beam arms; thus for each pair of R and λ, analyses were done for arm axial ratios (a/h) from 2.5 to 160. For these calculations, the adhesive properties were held constant at E 2 = 2500 MPa, ν 2 = 0.35, and α 2 = K 1 ; the adherend modulus was E 1 = RE 2 while ν 1 = 0.3 and α 1 = K 1 were held constant. The arm geometry (see Figures 1 and 2) was set to h = 5 mm and L = 2a = 2h(a/h); the analysis is independent of B. The composite beam was meshed into 8noded, isoparametric, quadrilateral elements with midside nodes. The energy release rate, G I, was calculated by crack closure methods [15]. With square cracktip elements, it was possible to get accurate results even with relatively coarse meshes. All results reported here were for a sufficiently refined mesh of about 600 elements and 2000 nodes. As expected, the errors in beamtheory C m and C r got larger as the arm axial ratio got smaller. At constant a/h, however, the relative errors in C m and C r were approximately independent of R and λ. The absolute value of the errors in C m or C r, averaged for λ from 1 to 128, are plotted as a function of a/h in Figure 3. Figure 3 is for R = 28 which corresponds to aluminum adherends (E 1 = MPa) with a typical epoxy adhesive (E 2 = 2500 MPa). The results for any other value of R (from 1 to 100) were similar, except that the errors for small a/h grew slightly at larger values of R. The errors in the residual stress coefficient, C r, were always less than 1% for a/h > 5 and were typically less than 0.01% for a/h > 10. For a/h < 5, the errors were still low for R < 20, but got larger and depended on λ for R > 20. Thus, except for the combination of a/h < 5 and R > 20, the simple beam theory result for C r does an excellent job of evaluating the contribution of residual stresses to total energy release rate.
6 64 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) Coefficient Error (%) C m Error C r Error Arm Axial Ratio (a/h) Fig. 3. The average or the absolute values of the errors between the theoretical coefficients C m and C r and the mechanical and residual stress results calculated by FEA as a function of the arm axial ratio. These results are for R = 28. For each arm axial ratio, the error was averaged for λ from 1 to 128. Because typical adhesive DCB specimens strive to use long, slender arms (large a/h), the residual stress correction evaluated here should be sufficiently accurate for all commonlyused adhesive fracture specimens. The errors in C m normally exceeded 1% and got very large for small a/h. This observed error in simple beam theory for calculating mechanical energy release rate has been discussed before [7 10]. The error is caused by an oversimplification in the simple beam theory analysis that prevents rotation of the specimen arms at the crack tip; for accurate analysis, this rotation can not be ignored. Williams analyzed an adhesive DCB specimen ignoring residual stresses [10]. He wrote a corrected mechanical beam theory result as G I ( T = 0) = (C m (a + W ) P ) 2 where C m = lim λ C m = 12 EB 2 h 3 1 is the limiting mechanical energy release rate coefficient for a very thin adhesive. In other words, the corrected analysis replaces the true crack length, a, by an effective crack length, a + W. Using the beamonelasticfoundation model of Kanninen [16], Williams derived the effective crack length correction in terms of specimen properties to be ( ) 1/4 1 + R λ W = h 1 (18) 6 If G F I EA is the energy release rate calculated by finite element analysis with T = 0, a numericallydetermined effective crack length correction for equation (17) can be found from F EA = (17) G F EA I C m P a (19) When including specimens with possibly thick adhesive layers, however, it is preferable to find the effective crack length correction relative to the full composite beam analysis for C m rather then for the thinadhesive beam result of C m. In other words, here the FEA effective crack length correction was found from F EA = G F EA I C m P a (20)
7 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) When this numericallycalculated F EA was compared to the theoretical W in equation (18) for all finite element calculations, they were found to be related by an almost constant ratio of F EA W = 1.15 (21) This ratio was independent of λ (in the range of 1 to 128) and a/h (in the range 2.5 to 160). The ratio was weakly dependent on R it was independent of R for R > 5 and increased slightly at low R, reaching 1.20 when R = 1. No attempt was made to derive the origin of the constant ratio of F EA to W. The beamonelastic foundation analysis in Ref. 10 ignored shear stresses although it was noted they could be added using the methods of Ref. 11. Because shear corrections depend on beam axial ratio while the results here were independent of arm axial ratio, it is unlikely that shear effects account for the discrepancy. Simple beam theory is one dimensional and thus does not account for Poisson ratio mismatch effects. To test for an effect of ν 1 ν 2 on the correction ratio, some additional calculations were done for R = 28 and ν 1 varying from to Again, there was no effect on the F EA / W ratio. The numerical result of 1.15 W can thus be regarded as a numericallydetermined correction factor valid for any typical adhesive DCB specimen with isotropic layers. Using the numericallydetermined adjustment to W, the energy release rate can be written as G I = ( (C m ) ) 2 W P a + C r T (22) a The average errors for all values of a/h 2.5 were less than 1% and typically much less than 1%. The maximum errors in the mechanical term occurred for small R while the maximum errors in the residual stress term occurred for large R. Even these maximum errors, however, were smaller than 1%, provided a/h Consequence of ignoring residual stresses Many previous adhesive toughness experiments have ignored residual stresses. The energy release rate result in equation (22) can be used to calculate the errors of such an approach. Assume that some particular adhesive has a true fracture toughness of G. If an adhesive DCB specimen with this adhesive is tested, it will fail when G I = G, which occurs when P = G C r T C m (a W ) (23) Notice that P < 0 if G < Cr 2 T 2. This condition corresponds to a DCB specimen that fails due to residual stresses alone. If the observed failure load is then used in an analysis that ignores residual stresses (equation (22) with T = 0), the apparent toughness and its percent error relative to the true G would be [ ( ) ( 2 G app = G C r T and G app Error = C ) ] 2 r T 1 (24) G This error, or consequence of ignoring residual stresses, can be calculated without knowledge of C m or W. For a sample calculation of errors due to ignoring residual stresses, we considered an adhesive with G = 200 J/m 2 and residual stresses due to α = K 1 and T = 100 C. These parameters correspond to a typical hightemperature cure epoxy adhesive bonded to metallic adherends. The total differential strain of α T = 0.40% is not excessively large for adhesive specimens. Because C r T < 0, G app will be higher than the true toughness. Figure 4 plots the percentage error in G app as a function of R for various λ from 2 to 64. The errors are extremely large for low R and low λ and decrease as either R or λ increase. In general, the errors are never insignificant. The dashed vertical line shows a typical R value for aluminumepoxy specimens (R = 28). Despite the high aluminumepoxy R value, the errors exceed 1% even with a very thin adhesive (λ = 64). The errors in aluminumepoxy specimens increase to over 40% as λ decreases to 2. Finally, the errors depend on total arm thickness (h). The results in Figure 4 were for h = 5 mm; the errors increase for specimens with larger h.
8 66 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) λ = 2 35 app G Error (%) λ = 8 λ = 4 C m Error (a/h=20) 15 λ = λ = 32 λ = Moduls Ratio (R = E 1 /E 2 ) Fig. 4. The error in G app when residual stresses are ignored as a function of R for various values of λ. The adhesive DCB specimens were assumed to have h = 5 mm, G = 200 J/m 2, α = K 1, and T = 100 C. The vertical dashed line corresponds to R = 28 which is a typical value for aluminumepoxy specimens. The nearlyhorizontal dashed line gives the errors caused in the mechanical energy release rate when ignoring the cracklength correction term for beam arms with a/h = 20. Early work on adhesive fracture using DCB specimens investigated the effects of adhesive joint thickness, DCB specimen width, and postcure temperature [1 3] on toughness, but these experiments ignored residual stresses and thus actually observed changes in G app instead of the true G. Interestingly, all experimentally observed trends in G app match predicted trends if we assume all changes are due solely to a change in level of residual stresses. As the adhesive joint gets thicker, λ get smaller which increases the residual stress effect and causes G app to increase; this prediction matches experiments [2, 3]. As the DCB specimen width changes, there should be no effect on G app ; this prediction matches experiments [3]. As the postcure temperature increases, T gets more negative, which increases the residual stresses and causes G app to increase; this prediction matches experiments [2, 3]. The magnitude of the observed G app changes with joint thickness and postcure temperature [2, 3] are probably larger than can be accounted for by a residual stress effect alone. It is likely, however, that residual stresses account for a nonnegligible fraction of the changes. The most appropriate physical picture of the changes in toughness should be derived from the true G instead of from G app. In one paper on postcure temperature effects, Mostovoy and Ripling [2] concluded that residual stresses are not important because G app increased with postcure temperature while they expected that an increased level of residual stress could only cause G app to decrease. This assessment is incorrect; in typical polymeric adhesives with metallic adherends, increasing the level of residual stresses causes G app to increase. Much effort has gone into corrections to the beamtheory mechanical term in proposing standards for mode I fracture of adhesive specimens [8, 10]. It is therefore interesting to compare the magnitude of the errors induced by ignoring the mechanical correction to those induced by ignoring residual stresses. If we consider a specimen with no residual stresses and a true toughness of G, by a similar procedure applied to analysis of residual stress errors, the percent error in the apparent toughness with respect to the true toughness caused by ignoring the mechanical term correction factor is [ ( ) 2 G app a Mechanical Error = 100 1] (25) a W This error is nearly independent of λ, but is a strong function of a/h and a weak function of R. Superimposed on Figure 4 is the mechanical error of typical adhesive specimens with a/h = 20. For an aluminum/epoxy specimen (R = 28), the residual stress error is larger than the mechanical error for thicker adhesives (λ < 10), but gets smaller for thinner adhesives (λ > 10). As a/h gets larger, the mechanical errors get smaller while
9 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) the residual stress errors do not change. Thus, for larger a/h, the residual stress errors will usually be larger than the mechanical errors. The exact value of the residual stress error depends on specimen geometry and the level of residual stresses in the adhesive, but in ordinary adhesive specimens it will often have a magnitude similar to the error induced by ignoring crack tip rotation. It makes little sense to carefully correct for all mechanical effects while ignoring a similarmagnitude residualstress error, especially since the residual stress effect can be accurately included by use of the C r T term in the energy release rate expression in equation (22) Asymptotic results for thin adhesives Many analyses of adhesive specimens assume the adhesive is thin. To judge the conditions for which the thinadhesive limit is valid, we derived asymptotic expansions for C m, C r, and W and compared those results to the full composite beam results. Expanding all results in a Taylor series in 1/λ and truncating after the linear terms gives the following asymptotic results: ( 12 C m (λ large) = E 1 B 2 h ) + O[1/λ 2 ] (26) 1 2Rλ C r (λ large) = α 3E1 h 1 + O[1/λ 2 ] (27) Rλ W (λ large) = h 1 ( 1 + R 4λ ) + O[1/λ 2 ] (28) The constant term in each limiting expression is the result as λ : Cm = lim C 12 m = λ E 1 B 2 h 3, Cr = lim C r = 0, and W = lim W = h 1 (29) 1 λ λ Notice that in the limit of no adhesive, there will be no beam curvature due to mismatched thermal expansion coefficients and thus the residual stress effect vanishes (Cr = 0). Figure 5 plots C m (λ large), Cm, C r (λ large), W (λ large), and W as a function of λ for a typical aluminumepoxy specimen. Each limiting result has been normalized to the full composite beam results in equations (15), (16), and (18) and thus deviations from 1 give the error caused by use of a limiting result rather than the full result. The limiting result Cr is not plotted because it is always zero. Both C m (λ large) and Cm converge very rapidly and agree within 1% with the full beam analysis, provided λ > 10. All other constants converge more slowly. C r (λ large) and W (λ large) require λ > 80 to be within 1% of the full beam analysis while W requires λ > 700. Figure 5 is for R = 28. The C m results converge faster as R gets larger while the W results converge slower. The C r convergence is relatively insensitive to R. In summary, it is acceptable to use thinadhesive, asymptotic results for C m, provided λ is larger than about 10 and R is not too small. For typical adhesive DCB specimens, however, it is not accurate to use the thinadhesive limits for either C r or W. The full expressions in equations (16) and (18) should be used instead. In other words, the fact that Cr = 0 or C r (λ large) is small does not imply that residual stresses can be ignored for thin adhesives Experimental suggestions By using equation (22) with C r determined by equation (16), it is possible to accurately determine G I for any typical adhesive DCB specimen including the effect of residual stresses. There are two experimental problems when correcting for residual stresses. First, evaluation of C r requires knowledge of α and T. Second, even if α and T are known, the form of C r in equation (16) assumes that both the adhesive and adherend are linear thermoelastic materials with temperatureindependent thermomechanical properties between T 0 and T s and that residual stresses are caused solely by differential thermal shrinkage. In real specimens, the thermomechanical properties will probably depend on temperature (especially in the adhesive near T 0 ) and there may be additional sources of residual stresses such as chemical shrinkage during adhesive cure. This section suggests some experimental methods for accounting for residual stresses that will be valid for any form of residual stresses.
10 68 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) W (λ large) Limiting Term/Full Term C m C m (λ large) W C r (λ large) λ Fig. 5. Plots of C m (λ large), C m, C r (λ large), W (λ large), and W as a function of λ. Each constant has been normalized the the full beam analysis results (C m, C r, and W ). These plots are for an aluminumepoxy specimen with R = 28 and h = 5 mm. By equation (5), each arm of the adhesive DCB specimen is assumed to have an effective momentcurvature relation. In the absence of mechanical loads, the curvature due to residual stresses is κ res = α κ T (30) To account for any type of residual stresses, we simply repeat the previous analysis but use κ res to calculate residual stress effects instead of α κ T. The result is that equations (7) and (8) change to where C res = κ res C κ B = κ resh 1 E 1 h 1 2λ 3 G I = (C m P a + C res ) 2 (31) ( 3(1 + λ) 2 + (1 + Rλ) λ 2 + Rλ Rλ The problem of accounting for residual stresses is reduced to experimentally finding κ res ; some possible experimental methods are illustrated in Figure 6. The method in Figure 6A is to construct a calibration specimen for each adhesive DCB specimen and subject it to identical adhesive cure conditions. The calibration specimen is a twolayer, adhesive and adherend strip. Such an unbalanced structure will curve due to residual stresses. By measuring the chord length, l, and strip height, d, the residual stress curvature can be calculated from [17] κ res = 2d (33) d 2 + l2 4 The sign of κ res is determined by the direction of curvature κ res is negative if the strip curves toward the adhesive and positive if it curves toward the adherend. Two drawbacks of using calibration specimens are that it requires preparing an extra specimen for each adhesive DCB specimen and that it may not be possible to subject the calibration specimens to identical cure conditions. Even when subjected to the same thermal history, the lack of an adherend on both sides of the adhesive may cause the calibration specimen to develop different residual stresses than the adhesive DCB specimen. Prior to a test, the arms of an adhesive DCB specimen with residual stresses will have some initial curvature caused by those stresses. Figures 6B and 6C show the possible types of initial arm curvature. This initial curvature could be used to determine κ res. This approach avoids the need for contruction of a ) (32)
11 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) l d A B C δ 0 δ 0 P D E h 2 δ int δ 2h 2 h 2 0 Fig. 6. Some experimental methods for determining the effect of residual stresses on G I in adhesive DCB specimens. A. Measure the curvature of an unbalanced, twolayer, adhesive and adherend strip. B. Measure initial arm curvature when κ res > 0. C. Measure initial arm curvature when κ res < 0. D. Determine intercept in loaddisplacement curve. E. Prepare symmetric specimens. second calibration specimen and guarantees that κ res is measured from the correct cure conditions. Figure 6B corresponds to a specimen with κ res > 0. For such specimens the arms will separate. From equation (6), the initial, total beam opening, δ 0, is related to κ res by δ 0 = a 2 κ res or κ res = δ 0 a 2 (34) Figure 6C corresponds to a specimen with κ res < 0. For such specimens, the arms will bend towards each other, but the arm ends will contact each other, inducing a load that prevents interpenetration. Integration of equation (5) and evaluation of the load P (M = P x) required for zero displacement at x = 0 shows that the maximum arm separation occurs at x = a/3. The maximum separation, δ 0, is related to κ res by δ 0 = 2a2 κ res 27 or κ res = 27δ 0 2a 2 (35) Notice that for specimens with identical magnitudes of κ res, the maximum arm separation used for determination of κ res is more than an order of magnitude smaller when κ res < 0 than it is when κ res > 0. This observation has two consequences. First, it may be difficult to accurately measure κ res when it is negative; this drawback is particularly troublesome because κ res is negative for most adhesive specimens. Second, an observation that there is not much initial curvature in the arms of an adhesive DCB specimen with κ res < 0 is not sufficient justification for ignoring residual stresses in that specimen. Perhaps a better way to measure κ res from the adhesive DCB specimen itself is to extract it from a measured loaddisplacement curve. Figure 6D shows an expected loaddisplacement curve where the displacement is the total arm displacement between the bottom surfaces of the arms measured at the loading points (x = 0). This curve is for an adhesive specimen with negative κ res ; the nonzero load at zero displacement is the load induced that prevents arm penetration. By extrapolation of the linear loaddisplacement curve with positive displacements to zero load, it is easy to show that the intercept, δ int, is related to κ res by δ int = a 2 κ res or κ res = δ int a 2 (36)
12 70 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) y 1 y 2 +h/2 h 1 h 2 E 1, α 1, θ 1 E 2, α 2, θ 2 B y x y n h/2 h n E n, α n, θ n Fig. 7. The coordinate system used for laminated beam analysis of one arm of an laminate DCB delamination specimen. The extrapolation methods works equally when for κ res > 0 and κ res < 0. The only difference is that when κ res < 0, the extrapolation must be done from positive displacements, which can be measured, into negative displacements, which cannot be measured. The only drawback of this interceptextrapolation method is that it requires the extra effort of accurately measuring beam opening during the experiments. The measured displacement must also be accurately calibrated to give zero displacement when the beam arms touch. Many adhesive specimens have an adhesive dropoff before the end of the specimen, as illustrated by the zone of length b in Figure 1. The extrapolation method can be modified to handle such specimens. Integration of the beam momentcurvature relation with allowance for a change in beam properties at x = b gives the intercept of the load displacement curve as δ int = 2h 2 + (a 2 b 2 )κ res or κ res = δ int 2h 2 a 2 b 2 (37) Here 2h 2 is the additional beam opening at the loading point because there is no adhesive present and the (a 2 b 2 ) term corrects for the reduced length of the zone with adhesive. When κ res < 0, the extrapolation must be made from displacements greater than 2h 2. The final experimental suggestion for dealing with residual stresses is to prepare specimens with no residual stress effect. As explained above, the entire effect of residual stresses can be traced to external work done by the arms as they curve due to the presence of residual stresses. This curvature can be eliminated by constructing symmetric DCB arms. As shown in Figure 6E, symmetric arms can be made by adding a layer of adhesive of thickness h 2 to both the top and bottom surfaces of the adhesive DCB specimen. The residual stresses can be ignored in the analysis of such a specimen. Three drawbacks of symmetric arms are that they complicate specimen fabrication, that the thickness of the outer layers must be carefully controlled to h 2 (or half to total adhesive joint thickness), and that the cure conditions must guarantee that the adhesive on the surfaces develop an identical level of residual stresses as the adhesive joint. 4. Laminate double cantilever beam specimens Another application of double cantilever beam specimens is to measure mode I delamination toughness of composite laminates [5]. By starting from equations (7) and (8), solving the laminate problem for energy release rate including the effect of residual stresses is simply a matter of determining Cκ and ακ for each arm of the laminate specimen. A simple laminated beam analysis of the single DCB arm in Figure 7 is given in the Appendix; substituting those results for Cκ and ακ into equation (8) gives the required C m and C r needed to for total G I. This planestress, laminate analysis treats the composite arms as beams. It therefore ignores possible anticlastic curvature and bendingtwisting coupling effects [18, 19]. As with adhesive DCB specimens, the simple beam theory result for C m is not very accurate and needs to be corrected for beam rotation effects. As with the adhesive DCB specimen, that correction can be done by introducing an effective crack length as has been discussed by Williams [11]. Because laminate DCB arms are orthotropic materials, the C m correction differs from the one for adhesive DCB specimen with isotropic arms [11]. The remainder of this section will only consider the effects of residual stresses and suggest experimental methods for accounting for residual stresses. Each of these topics can be analyzed accurately without knowledge of the correction factors required for C m.
13 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) Table 1. Errors caused by ignoring residual stresses in delamination experiments on a series of graphite/epoxy laminates. The experiments are assumed to be on 16ply laminates with delamination in the middle of the laminate. The laminates listed here are the layups for the 8ply laminates in each DCB specimens. 8Ply Arm G IC Error 8Ply Arm Layup G IC Error (%) Layup (%) [0 8 ] 0.00 [0 2 /90 2 /0 2 /90 2 ] [90/0 7 ] [0/90/0/90/0/90/0/90] [90 2 /0 6 ] [90/0/90/0/90/0/90/0] [90 4 /0 4 ] [90 2 /0 2 /90 2 /0 2 ] [90 6 /0 2 ] [0 2 /90 2 /45 2 / 45 2 ] [90 8 ] 0.00 [90 2 /0 2 /45 2 / 45 2 ] [0 2 /90 6 ] [0 2 /45 2 / 45 2 /90 2 ] [0 4 /90 4 ] [90 2 /45 2 / 45 2 /0 2 ] [0 6 /90 2 ] [45 2 / 45 2 /0 2 /90 2 ] [0 7 /90] [ 45 2 /45 2 /90 2 /0 2 ] Consequence of ignoring residual stresses From equation (24), the error caused by ignoring residual stresses is a function only of C r, T, and G IC. We considered a series of graphite/epoxy laminates with G IC = 200 J/m 2 and T = 125 C, which are typical values for graphite epoxy laminates [20 22]. The value of C r depends on the layup of the specimen arms and can be calculated by the laminated beam analysis in the Appendix followed by substitution into equation (8). Table 1 lists the error caused by ignoring residual stresses for delamination down the middle of a series of 16ply laminates which leads to 8ply laminate DCB arms. In all examples, the undelaminated 16 ply laminate is symmetric; the 8ply arms, however, may be unsymmetric. The ply properties used in these calculations were E 1 = MPa, E 2 = 8970 MPa, ν 12 = 0.30, G 12 = 6900 MPa, α 1 = K 1, α 2 = K 1, and h i = mm. The first column of Table 1 gives a series of DCB arms with 0 and 90 plies. The two special cases of [0 8 ] and [90 8 ] are not affected by residual stresses and thus introduce no error. The arms in these specimens are themselves symmetric laminates and therefore do not curve due to residual stresses. Because there is no thermal curvature, there is no external work due to residual stresses and no residual stress effect on G I. These layups will have residual stresses caused by differential shrinkage between the fibers and the matrix. These residual stresses, however, do not release any energy as the delamination crack propagates. Many previous delamination experiments have been done on unidirectional laminates. It is correct to ignore residual stresses when analyzing such experiments. All other arrangements of 0 and 90 plies, besides [0 8 ] and [90 8 ], have an effect of residual stresses that cannot be ignored. The smallest error, caused by a change of a single ply on the surface, is 6.21% ([90/0 7 ]); the largest error is 76.36% ([0 2 /90 6 ]). An interesting example is the [0 4 /90 4 ] laminate. If the delamination growth is parallel to the fibers in the surface plies, the apparent G IC will be 46.54% too high (293 J/m 2 in this example). But, if the laminate is rotated 90 and the delamination is propagated parallel to the fibers in the central plies, the apparent G IC will be 37.68% too low (125 J/m 2 in this example). The two apparent toughnesses will differ by more than a factor of two. The second column of Table 1 lists some alternate layups with four 0 and four 90 plies and lists some quasiisotropic layups. Among the 0/90 laminates, the sign of the error depends on the stacking sequence and the magnitude depends on the ply groupings. Positive errors result when the 90 plies are in the middle while negative errors result when 0 plies are in the middle. The errors get smaller as the ply groupings get smaller; the smallest error is for alternating 0 and 90 plies. Among the quasiisotropic layups, the error ranges from % to %. It is not possible to construct laminate arms made from 0 2, 90 2, 45 2, and 45 2 ply pairs having a residual stress effect that causes less than a 14% error. If the ply pairs are split apart, the errors can be made smaller. Symmetric arm layups such as [0/90/ + 45/ 45/ 45/ + 45/90/0]
14 72 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) would have no residual stress effects Experimental suggestions Rather than calculate C r from laminated plate or beam theory and knowledge of T, it is preferable to experimentally correct for residual stresses. As with adhesive DCB specimens, experimental correction avoids having to measure additional thermomechanical properties and furthermore can account for residual stresses caused by any mechanisms. As with adhesive DCB specimens, residual stress curvature in laminate DCB specimens can be evaluated by using calibration specimens (Figure 6A), by measuring initial arm curvature (Figures 6B and 6C), or by extrapolating from carefullyzeroed, loaddisplacement results (Figure 6D). The extrapolation method is probably the best method. Also like adhesive DCB specimens, the residual stress effect can be eliminated by use of specimens with symmetric arms [18, 19] (Figure 6E). This approach is more attractive in delamination specimens than in adhesive specimens because instead of the extra work of adding layers and carefully controlling their thickness, it only requires selecting specimens with a doublysymmetric layup. Here, a doublesymmetric layup is a symmetric laminate for which each delaminating arm is itself a symmetric laminate. The absence of a residual stress effect in doublysymmetric laminates assumes the laminate was cooled slow enough such that there are no residual stresses due to thermal gradients during cooling. A specimen that is cooled rapidly would probably develop compressive stresses on the surface and tensile stresses in the middle. Such a distribution of residual stresses would cause the arms to curve away from each other as they delaminate or act like a specimen with κ res > 0 and give an apparent toughness that is lower than the true toughness. Because thermal gradient effects become larger as the laminate gets thicker, compression on the outside and tension in the middle would cause the toughness to decrease as the specimens get thicker. Because the axial thermal expansion coefficient of many unidirectional carbonfiber laminates is negative, an opposite situation would occur for delamination parallel to the fibers. Rapid cooling would cause tension on the outside and compression in the middle and the apparent toughness would increase as the specimens got thicker. Indeed, the apparent toughness of unidirectional IM6 carbon fiber/peek specimens has been observed to increase with arm thickness [23]. This observation, however, was attributed to fiber bridging instead of residual stresses [23]. That conclusion is supported by the extra experiments in Ref. 23 that showed that the toughness did not change as the cooling rate increased. Acknowledgements This work was supported by a grant from the Mechanics of Materials program at the National Science Foundation CMS Appendix A The effective properties of a laminate DCB specimen can be determined from laminated plate theory. Here, however, all analyses are planestress, beam analyses and therefore a laminated beam theory was used. For the laminate arm illustrated in Figure 7 under axial strain ε 0 and curvature κ, the axial strain as a function of y is ε(y) = ε 0 κy (38) where κ > 0 corresponds to curvature upward. The axial stress in each layer, including residual stresses, is σ(y) = E(y) ( ε 0 κy α(y) T ) (39) where E(y) and α(y) are the positiondependent modulus and thermal expansion coefficient in the x direction. Integrating these stresses, the total axial force, F, and bending moment, M, can be written as F = A 11 ε 0 B 11 κ N T T and M = B 11 ε 0 + D 11 κ + M T T (40)
15 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) where h/2 A 11 = B E(y)dy = B h/2 h/2 B 11 = B y E(y)dy = B h/2 n E(θ i )h i (41) i=1 h/2 D 11 = B y 2 E(y)dy = B h/2 n E(θ i )h i ȳ i (42) i=1 h/2 N T = B E(y)α(y)dy = B h/2 n ( ) E(θ i )h i ȳ 2 i + h2 i (43) 12 n E(θ i )α(θ i )h i (44) i=1 h/2 M T = B y E(y)α(y)dy = B h/2 i=1 n E(θ i )α(θ i )h i ȳ i (45) i=1 (46) Here E(θ i ), α(θ i ), h i, and ȳ i are the xdirection modulus, xdirection thermal expansion coefficient, thickness, and midpoint of ply i with orientation angle θ i. A 11, B 11, and D 11 are the (1, 1) elements of the usual laminated plate theory A, B, and D matrices except for the extra factor of B because F and M are total forces and moments instead of force and moment resultants. By the usual rules for rotation of thermomechanical properties, E(θ i ) and α(θ i ) are 1 E(θ i ) ( = cos4 θ i 1 + 2ν ) 12 sin 2 θ i cos 2 θ i + sin4 θ i (47) E 1 G 12 E 1 E 2 α(θ i ) = α 1 cos 2 θ i + α 2 sin 2 θ i (48) Here E 1, E 2, G 12, ν 12, α 1, and α 2 are the inplane tensile and shear moduli, Poisson s ratio, and thermal expansion coefficients of the ply material with 1 being the fiber direction and 2 being the transverse direction. Finally, setting F = 0 and solving for κ gives where the effective beam properties are κ = C κm + α κ T (49) A 11 Cκ = A 11 D 11 B11 2 and α κ = B 11N T A 11 M T A 11 D 11 B 2 11 (50) References [1] Ripling, E. J., S. Mostovoy, and R. L. Patrick Materials Research & Standards 1964, 4, [2] Mostovoy, S. and E. J. Ripling J. Appl. Polym. Sci. 1966, 10, [3] Mostovoy, S. and E. J. Ripling J. Appl. Polymer Sci. 1971, 15, [4] ASTM D , in Annual Book of ASTM Standards 1996, 15.06, [5] ASTM D a, in Annual Book of ASTM Standards 1996, 15.03, [6] Reeder, J. R. and J. H. Crews, Jr. AIAA J. 1990, 28, [7] Hashemi, S., A. J. Kinloch, and J. G. Williams Proc. R. Soc. Lond. 1990, A347, [8] Blackman, B., A. J. Kinloch, and J. G. Williams, personal communication. [9] Williams, J. G. J. Comp. Mater. 1987, 21, [10] Williams, J. G. in Proc. Int l Mechanical Engineering Congress and Exhibition: The Winter Annual Meeting of the ASME, Symposium on Mechanics of Plastics and Plastic Composites November 1995, San Francisco, USA. [11] Williams, J. G. Comp. Sci. & Tech. 1989, 35,
16 74 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) [12] Nairn, J. A. J. Applied Mech. 1997, 64, [13] Crandall, S. H., N. C. Dahl, and T. J. Lardner, An Introduction to the Mechanics of Solids, McGraw Hill Book Company, New York (1978). [14] Timoshenko, S. J. Opt. Soc. Amer. 1925, 11, [15] Krishnamurthy, T., Ramamurthy, T. S., Vijayakumar, K. and Dattaguru, B. in Proc. Int. Conf. Finite Elements in Computational Mechanics, 26 December 1985, Bombay, India, [16] Kanninen, M. F. Int. J. Fract. 1973, 9, [17] Nairn, J. A. and P. Zoller ASTM STP , [18] Hudson, R. C., B. D. Davidson, and J. J. Polaha Proc. ICCM , I, [19] Polaha, J. J., B. D. Davidson, R. C. Hudson, and A. Pieracci J. Reinforced Plast. and Comp. 1996, 15, [20] Hunston, D. L. Comp. Tech. Rev. 1984, 6, [21] Hunston, D. L., R. J. Moulton, N. J. Johnston, and W. D. Bascom in Toughened Composites, ed. N. J. Johnston 1987, ASTM STP 937, [22] Liu, S. and J. A. Nairn J. Reinf. Plast. & Comp. 1992, 11, [23] Davies, P., W. Cantwell, C. Moulin, and H. H. Kausch Comp. Sci. & Tech. 1989, 36,
Fracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationOn the calculation of energy release rates for cracked laminates with residual stresses
International Journal of Fracture, 39, 67 93 006) On the calculation of energy release rates for cracked laminates with residual stresses J. A. NAIRN Wood Science and Engineering, Oregon State University,
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments
Engineering Fracture Mechanics ) 4 Author prepared preprint Fracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments SungRyong Kim a, John A. airn
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationA PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS
1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationAnalytical and experimental methods for a fracture mechanics interpretation of the microbond test including the effects friction and thermal stresses
International Journal of Adhesion & Adhesives 19 (1999) 59 7 Analytical and experimental methods for a fracture mechanics interpretation of the microbond test including the effects friction and thermal
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationFRACTURE MECHANICS IN ANSYS R16. Session 04 Fracture Mechanics using Cohesive Zone Material (CZM) Model
FRACTURE MECHANICS IN ANSYS R16 Session 04 Fracture Mechanics using Cohesive Zone Material (CZM) Model COHESIVE ZONE MATERIAL MODEL (CZM) Fracture or delamination along an interface between phases plays
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 6 Fracture Toughness Testing and Residual
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationEVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES
EVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES Koji YAMAGUCHI 1, Isao KIMPARA 1, and Kazuro KAGEYAMA 1 1 Department of Environmental &
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationDynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites
Engineering Fracture Mechanics 7 (5) 53 558 www.elsevier.com/locate/engfracmech Dynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites Sylvanus
More informationValidity of fracture mechanics concepts applied to wood by finite element calculation
Wood Sci. Technol. 18:5158 (1984) Wood Science and Technology 9 SpringerVerlag 1984 Validity of fracture mechanics concepts applied to wood by finite element calculation P. Triboulot*, Champenoux, P.
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationBRIDGED DELAMINATION CRACKS IN CURVED BEAMS AND MIXEDMODE BENDING SPECIMENS
BRDGED DELANATON CRACKS N CURVED BEAS AND XEDODE BENDNG SPECENS Roberta assabò and Brian N. Cox Department of Structural and Geotechnical Engineering, University of Genova, Via ontallegro, 645, Genova,
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More informationIMECE CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT
Proceedings of IMECE04 2004 ASME International Mechanical Engineering Congress November 1320, 2004, Anaheim, California USA IMECE200460700 CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT Jianzheng Zuo Department
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationMassachusetts Institute of Technology 22.68J/2.64J Superconducting Magnets. February 27, Lecture #4 Magnetic Forces and Stresses
Massachusetts Institute of Technology.68J/.64J Superconducting Magnets February 7, 003 Lecture #4 Magnetic Forces and Stresses 1 Forces For a solenoid, energy stored in the magnetic field acts equivalent
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationDELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE
DELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE F. LACHAUD 1,2, R. PIQUET 2, L. MICHEL 1 2 LMT, IUT de énie Mécanique, 50, Chemin des Maraîchers, 31077 TOULOUSE
More informationElasticPlastic Fracture Mechanics. Professor S. Suresh
ElasticPlastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationTHE demand for plastic packages has increased due to
294 IEEE TRANSACTIONS ON COMPONENTS AND PACKAGING TECHNOLOGIES, VOL. 30, NO. 2, JUNE 2007 Predictive Model for Optimized Design Parameters in FlipChip Packages and Assemblies Seungbae Park, H. C. Lee,
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationDiscontinuous Distributions in Mechanics of Materials
Discontinuous Distributions in Mechanics of Materials J.E. Akin, Rice University 1. Introduction The study of the mechanics of materials continues to change slowly. The student needs to learn about software
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationMultiscale modeling of failure in ABS materials
Institute of Mechanics Multiscale modeling of failure in ABS materials Martin Helbig, Thomas Seelig 15. International Conference on Deformation, Yield and Fracture of Polymers Kerkrade, April 2012 Institute
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationAvailable online at ScienceDirect. 20th European Conference on Fracture (ECF20) Yu.G. Matvienko*
Available online at www.sciencedirect.com ScienceDirect Procedia Materials Science 3 ( 014 ) 141 146 0th European Conference on Fracture (ECF0) The Effect of the nonsingular Tstress components on crack
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationComputer Methods in Applied Mechanics and Engineering, 66, (1988).
1 FINITE ELEMENT ANALYSIS OF STRESS CONCENTRATION AROUND A BLUNT CRACK IN A COSSERAT ELASTIC SOLID S. Nakamura and R.S. Lakes adapted from Computer Methods in Applied Mechanics and Engineering, 66, 257266
More informationCracks Jacques Besson
Jacques Besson Centre des Matériaux UMR 7633 Mines ParisTech PSL Research University Institut Mines Télécom Aγνωστ oς Θεoς Outline 1 Some definitions 2 in a linear elastic material 3 in a plastic material
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationThe Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials under Kinematic Harmonic Loading
Mechanics and Mechanical Engineering Vol. 21, No. 1 (2017) 157 170 c Lodz University of Technology The Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationProgram: Recent Trends
The SNL/MSU/DOE Fatigue Program: Recent Trends John Mandell Montana State University 2012 SNL Blade Workshop May 30  June 1, 2012 Outline Overview of MSU Fatigue Program on Wind Blade Materials: Testing
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationIndeterminate Analysis Force Method 1
Indeterminate Analysis Force Method 1 The force (flexibility) method expresses the relationships between displacements and forces that exist in a structure. Primary objective of the force method is to
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationDelamination in the scoring and folding of paperboard
PEERREVIEWED CONVERTING Delamination in the scoring and folding of paperboard DOEUNG D. CHOI, SERGIY A. LAVRYKOV, and BANDARU V. RAMARAO ABSTRACT: Delamination between layers occurs during the creasing
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More information